Gold Network Structures in Rhombohedral and Monoclinic Sr2Au6(Au,T)3 (T = Zn, Ga). A Transition via Relaxation
Trinath Mishra; Qisheng Lin; John D. Corbett; Inorganic Chemistry 52 (2013) 13623–13630; doi:10.1021/ic402145k

data_4336887
_publ_section_title
;
 Gold Network Structures in Rhombohedral and Monoclinic Sr2Au6(Au,T)3 (T =
 Zn, Ga). A Transition via Relaxation
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              13623
_journal_page_last               13630
_journal_paper_doi               10.1021/ic402145k
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Au6.82 Sr2 Zn2.18'
_chemical_formula_weight         1660.40
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 123.450(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   14.6833(7)
_cell_length_b                   8.4649(4)
_cell_length_c                   8.7463(4)
_cell_measurement_reflns_used    9496
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.99
_cell_measurement_theta_min      2.92
_cell_volume                     907.04(8)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'bruker Apex2 CCD'
_diffrn_measurement_method       w/
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0849
_diffrn_reflns_av_sigmaI/netI    0.0513
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            9496
_diffrn_reflns_theta_full        29.99
_diffrn_reflns_theta_max         29.99
_diffrn_reflns_theta_min         2.92
_exptl_absorpt_coefficient_mu    126.985
_exptl_absorpt_correction_T_max  0.7476
_exptl_absorpt_correction_T_min  0.4061
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            grey
_exptl_crystal_density_diffrn    12.159
_exptl_crystal_description       irregular
_exptl_crystal_F_000             2720
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_refine_diff_density_max         5.947
_refine_diff_density_min         -3.850
_refine_diff_density_rms         0.906
_refine_ls_extinction_coef       0.00042(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.126
_refine_ls_matrix_type           full
_refine_ls_number_parameters     54
_refine_ls_number_reflns         1323
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.126
_refine_ls_R_factor_all          0.0554
_refine_ls_R_factor_gt           0.0465
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0359P)^2^+196.4147P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1061
_refine_ls_wR_factor_ref         0.1093
_reflns_number_gt                1135
_reflns_number_total             1323
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic402145k_si_003_5.cif
_cod_data_source_block           crystal_5_Sr2Au6.82Zn2.18
_cod_original_cell_volume        907.04(7)
_cod_database_code               4336887